# UCI Physics and Astronomy - Intermediate valence metals jmlawren/IV_UCI06.pdf¢ ...

date post

14-Jul-2020Category

## Documents

view

3download

0

Embed Size (px)

### Transcript of UCI Physics and Astronomy - Intermediate valence metals jmlawren/IV_UCI06.pdf¢ ...

1

Intermediate valence metals Jon Lawrence, UCI Colloquium, 12 October 2006

www.physics.uci.edu/~jmlawren 1. Introduction to concept of intermediate valence (IV) 2. Anderson impurity model Fits of χ(T), nf(T), Cp(T), χ’’(ω) to AIM (dominated by local spin fluctuations) PES(w) showing large vs. small energy scales 3. Coherent Fermi liquid ground state: Transport, specific heat and Pauli susceptibility De Haas van Alphen and LDA band theory Optical conductivity, neutron scattering and the Anderson Lattice 4. Anomalies Slow crossover from Fermi liquid to local moment Low temperature susceptibility and specific heat anomalies Low temperature anomaly in the spin dynamics

Collaborators: LANL CMP: Zach Fisk, Joe Thompson, John Sarrao, Mike Hundley, Al Arko, George Kwei, Eric Bauer NHMFL/LANL: Alex Lacerda, Neil Harrison Argonne National Lab: Ray Osborn, Eugene Goremychkin Brookhaven National Lab: Steve Shapiro Shizuoka University: Takao Ebihara UCI Postdocs: Andy Cornelius (UNLV), Corwin Booth (LBL), Andy Christianson (ORNL) UCI students: Jerry Tang, Victor Fanelli Temple U.: Peter Riseborough

2

Intermediate Valence Compounds

CeBe13 Fermi liquid (FL) YbAgCu4 CePd3 FL with anomalies YbAl3 Ce3Bi4Pt3 Kondo Insulator YbB12 γ-α Ce Valence transition YbInCu4

Intermediate Valence (IV) = Nonintegral valence

Yb: (5d6s)3 4f13 nf = 1 trivalent (5d6s)2 4f14 nf = 0 divalent

YbAl3 (5d6s)2.75 4f13.25 nf = 0.75 IV

Ce: (5d6s)34f1 nf = 1 trivalent (5d6s)44f0 nf = 0 tetravalent

CePd3 (5d6s)3.24f0.8 nf = 0.8 IV

Oversimplified single ion model:

Two nearly-degenerate localized configurations form hybridized w.f.:

a [4f13(5d6s)3> + b [4f14(5d6s)2> where a = √nf and b = √(1 – nf)

3

These IV properties are captured by Anderson Impurity Model (AIM)Basic underlying physics:

Highly localized 4f13 orbital surrounded by a sea of conduction electrons

Nearly degenerate with 4f14 orbital Energy separation: Ef

Strong on-site Coulomb interaction U between 4f electrons; 4f12 orbital at energy Ef + U where U >> V, Ef

Hybridization V between configurations: conduction electrons hop on and off the 4f impurity orbital. Hybridization strength Γ = V2ρ where ρ is the density of final (conduction) states.

Correlated hopping: when Γ ~ Ef

4

Key predictions of Anderson Impurity model: Energy lowering due to hybridization:

kBTK ~εF exp{-Ef/[NJ V2 ρ(εF)]} ~ (1 – nf) NJ V2 ρ(εF) Kondo Resonance: Narrow 4f resonance at the Fermi level εF.

(Virtual charge fluctuations yield low energy spin fluctuations.) Contributes to the density-of-states (DOS) as ρf(εF) ~ 1/TK.

Mixed valence due to hybridization (nf < 1) Spin/valence fluctuation: localized, damped oscillator with characteristic energy

E0 = kBTK : χ’’~ χ (T) E Γ/((E-E0)2 + Γ 2) Universality: Properties scale as T/TK, E/kBTK, μBH/kBTK

High temperature limit: LOCAL MOMENT PARAMAGNET Integral valence: nf → 1 z = 2+nf = 3 Yb 4f13(5d6s)3

Curie Law: χ → CJ/T where CJ = N g2 μB2 J(J+1)/ 3 kB J = 7/2 (Yb) Full moment entropy: S → R ln(2J+1)

CROSSOVER at Characteristic temperature TK Low temperature limit: FERMI LIQUID Nonintegral valence (nf < 1) Yb 4f14-nf (5d6s)2+nf

Pauli paramagnet: χ(0) ~ μB2 ρf(εF) Linear specific heat: Cv ~ γ T γ = (1/3) π2 ρf(εF) kB2

All approximately valid for periodic IV metals.

5

Q-dependence: In YbInCu4 (Lawrence, Shapiro et al, PRB 55 (1997) 14467) no dependence of Γ or E0 on Q and only a weak (15%) dependence of χ’ on Q.

Q-independent, broad Lorentzian response ⇒

Primary excitation is a local, highly damped spin fluctuation (oscillation) at characteristic energy E0 = kBTK

Lawrence, Osborn et al PRB 59 (1999) 1134

YbInCu4 Magnetic scattering Smag vs. E at two incident energies Ei

E

Spin fluctuation spectra YbInCu4

Lorentzian power spectrum

S(E) ~ χ’ E P(E) = χ’ E (Γ/2)/{(E - E0)2 + Γ2}

6

0.00

0.01

0.02

0 100 200 300

0 5 10 15 20 0

10

20

T(K) YbAgCu4 Data Theory: W = 0.865 Ef = -0.4485 V = 0.148 TK(K) = 95K

χ( em

u/ m

ol )

0.8

0.9

1.0

n f

S (m

b/ sr

-m eV

)

ΔE(meV)

Fits to the AIM YbAgCu4: Good quantitative fits

to the T dependence of χ, nf, γ and to the low T neutron spectrum

O data ___ AIM

Lawrence, Cornelius, Booth, et al

Two parameters (Ef, V) chosen to fit χ(0) and nf(0)

(plus one parameter for background bandwidth W, chosen to agree with specific heat of nonmagnetic analogue LuAgCu4)

7

Comparison to AIM YbAl3: Semiquantitative

agreement

AIM parameters

(Chosen to fit χ(0), nf(0) and γ(LuAl3))

W = 4.33eV Ef = -0.58264eV V = 0.3425eV TK = 670K

Cornelius et al PRL 88 (2002) 117201

The AIM predictions evolve more slowly with temperature than the data (slow crossover between the Fermi liquid and the

local moment regime) and there are low temperature anomalies in the susceptibility, specific heat and the neutron spectrum.

8

Comparison to AIM (continued) YbAl3 Spin dynamics: Neutron scattering (Q- averaged)

At T = 100K the neutron scattering exhibits an inelastic (IE) Kondo peak:

χ’’(E) = Γ E / ((E- E1)2 + Γ2)

representing the strongly damped local excitation. For YbAl3, E1/kB = 550 K which is of order TK.

This Lorentzian is still present at 6 K where experiment gives

E1 = 50 meV and Γ = 18 meV while the AIM calculation gives

E1 = 40meV and Γ = 22meV (Semiquantitative agreement)

In addition, there is a new peak (low temperature anomaly) at 32 meV.

Lawrence, Christianson et al, unpublished data

9

5 4 3 2 1 0 Binding Energy (eV)

The AIM prediction for photoemission (Gives the relationship between

large and small energy scales)

Primary 4f1 → 4f0 emission at –Ef ~ (-2.7 eV in CeBe13)

Hybridization width 1 eV = NJ V2 ρ(εF) {implies exp[-Ef/ (NJ V2 ρ(εF))] = 0.066}

Kondo Resonance near Fermi energy εF w/ width proportional to TK.

Qualitative agreement, but there is a long- standing argument about the details:

E.g. the relative weight in the KR is larger than expected, suggesting the 4f electrons are forming narrow bands near εF.

The temperature dependence is also not as predicted, (perhaps “slow crossover” )

Many problems arise from the high surface sensitivity of the measurement.Lawrence, Arko et al PRB 47 (1993) 15460

10

TRANSPORT BEHAVIOR OF IV COMPOUNDS

The AIM predicts a finite resistivity at T = 0 due to unitary scattering from the 4f impurity.

In an IV compound, where the 4f atoms form a periodic array, the resistivity must vanish. (Bloch’s law)

Typically in IV compounds ρ ~ A (T/T0)2

This is a sign of Fermi Liquid “coherence” among the spin fluctuations.

YbAl3 ρ vs T2

↓

Ebihara et al Physica B 281&282 (2000) 754

11

C/T vs. T2 for YbAl3

Ebihara et al Physica B 281&282 (2000) 754

FERMI LIQUID BEHAVIOR A Fermi liquid is a metal where, despite the strong electron-electron interactions, the statistics at low T are those of a free (noninteracting) Fermi gas, but with the replacement m → m* (the effective mass). The specific heat is linear in temperature C = γ T

γ = {π2 kB2 NA Z/(3 h3 π2 N/V)2/3)} m*

For simple metals (e.g. K): γ = 2 mJ/mol-K2 m* = 1.25 me

For YbAl3: γ = 45 mJ/mol-K2 m* ~ 25 me

→ “Moderately HEAVY FERMION” compound

γ = 45 mJ/mol-K2

The Fermi liquid also exhibits Pauli paramagnetism:

YbAl3: χ(0) = 0.005 emu/mol

12

The AIM is qualitatively good (and sometimes quantitatively, e.g. YbAgCu4) for χ (T), Cv(T), nf(T) and χ’’(ω;T)

essentially because these quantities are dominated by spin fluctuations, which are highly local.

BUT: to get the correct transport behavior and the coherent Fermi Liquid behavior ⇒ Theory must treat the 4f lattice

Two theoretical approaches to the Fermi Liquid State Band theory: Itinerant 4f electrons: Calculate band structure in the LDA.

One-electron band theory (LDA) treats 4f electrons as itinerant; it does a good job of treating the 4f-conduction electron hybridization.

It correctly predicts the topology of the Fermi surface. But: Band theory strongly underestimates the effective masses!

LDA: m* ~ me dHvA: m*~ 15-25 me And, it can’t calculate the temperature dependence.

Anderson Lattice Model: Localized 4f electrons Put 4f electrons, with AIM interactions (Ef, V, U), on each site of a periodic lattice.

This loses the details of the Fermi surface but gets the effective masses and the T-dependence correctly.

Bloch’s law is satisfied for both cases.

13

De Haas van Alphen and the Fermi surface Figures from Ebihara et al, J Phys Soc Japan 69 (2000) 895

The de Haas van Alphen experiment m

*View more*